LMucko/crystallography-open-database huggingface dataset:
The crystal structures of some Vernier phases in the yttrium oxide-fluoride system
Bevan, D. J. M.; Mohyla, J.; Hoskins, B. F.; Steen, R. J.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 451–465; doi:

data_4030263
_publ_section_title
;
 The crystal structures of some Vernier phases in the yttrium
 oxide-fluoride system
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              451
_journal_page_last               465
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'F9 O6 Y7'
_chemical_formula_weight         889.37
_space_group_IT_number           39
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      39
_symmetry_space_group_name_Hall  'A 2 -2b'
_symmetry_space_group_name_H-M   'A b m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.423(1)
_cell_length_b                   38.624(6)
_cell_length_c                   5.527(1)
_cell_volume                     1157.7(3)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.542
_exptl_absorpt_coefficient_mu    4.755
_exptl_crystal_density_diffrn    5.10
_refine_ls_number_parameters     36
_refine_ls_number_reflns         418
_refine_ls_R_factor_gt           0.054
_refine_ls_wR_factor_gt          0.048
_cod_data_source_file            EJSSIC-1990-27-451-465-3.cif
_cod_data_source_block           Y7O6F9
_cod_original_sg_symbol_Hall     'A 2 -2c'
_cod_database_code               4030263
The crystal structures of some Vernier phases in the yttrium oxide-fluoride system
Bevan, D. J. M.; Mohyla, J.; Hoskins, B. F.; Steen, R. J.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 451–465; doi:

data_4030264
_publ_section_title
;
 The crystal structures of some Vernier phases in the yttrium
 oxide-fluoride system
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              451
_journal_page_last               465
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'F23 O14 Y17'
_chemical_formula_weight         2172.36
_space_group_IT_number           39
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      39
_symmetry_space_group_name_Hall  'A 2 -2b'
_symmetry_space_group_name_H-M   'A b m 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.413(1)
_cell_length_b                   93.917(6)
_cell_length_c                   5.529(1)
_cell_volume                     2810.8(7)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.542
_exptl_absorpt_coefficient_mu    4.762
_exptl_crystal_density_diffrn    5.13
_refine_ls_number_parameters     84
_refine_ls_number_reflns         687
_refine_ls_R_factor_gt           0.101
_refine_ls_wR_factor_gt          0.116
_cod_data_source_file            EJSSIC-1990-27-451-465-4.cif
_cod_data_source_block           Y17O14F23
_cod_original_sg_symbol_Hall     'A 2 -2c'
_cod_database_code               4030264
The crystal structure of Na2CuFeF7, a new variant in the weberite family
Yacubovich, O. V.; Urusov, V. S.; Frenzen, G.; Massa, W.; Babel, D.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 467–475; doi:

data_4030265
_publ_section_title
;
 The crystal structure of Na2CuFeF7, a new variant in the weberite family
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              467
_journal_page_last               475
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'Cu F7 Fe Na2'
_chemical_formula_weight         298.38
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.36(7)
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.46(1)
_cell_length_b                   7.363(8)
_cell_length_c                   12.93(1)
_cell_volume                     1119.2(18)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    6.621
_exptl_crystal_density_diffrn    3.542
_exptl_crystal_F_000             1120
_refine_ls_number_parameters     108
_refine_ls_number_reflns         2042
_refine_ls_R_factor_gt           0.0294
_refine_ls_wR_factor_gt          0.0276
_cod_data_source_file            EJSSIC-1990-27-467-475.cif
_cod_data_source_block           Na2CuFeF7
_cod_original_sg_symbol_H-M      'C 2/c'
_cod_database_code               4030265
Preparation, structure determination and transport properties of a new misfit layer compound : (PbS1.14)(NbS2)2
Meerschaut, A.; Guemas, L.; Auriel, C.; Rouxel, J.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 557–570; doi:

data_4030266
_publ_section_title
;
 Preparation, structure determination and transport properties of a new
 misfit layer compound : (PbS1.14)(NbS2)2
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              557
_journal_page_last               570
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'Nb2 Pb1.14 S5.14'
_chemical_formula_weight         586.835
_space_group_IT_number           36
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      36
_symmetry_space_group_name_Hall  'C 2c -2'
_symmetry_space_group_name_H-M   'C m c 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.3263(9)
_cell_length_b                   5.776(2)
_cell_length_c                   35.876(13)
_cell_volume                     689.3(4)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    30.996
_exptl_crystal_density_diffrn    5.517
_refine_ls_number_parameters     20
_refine_ls_number_reflns         137
_refine_ls_R_factor_gt           0.054
_refine_ls_wR_factor_gt          0.066
_cod_data_source_file            EJSSIC-1990-27-557-570.cif
_cod_data_source_block           (PbS1.14)(NbS2)2
_cod_database_code               4030266
Synthesis and structure of new n5-pentamethylcyclopentadienyldimethylplatinum (IV) complexes
Rockensuss, W.; Roeski, H. W.; Gilje, J. W.; Noltemeyer, M.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 599–615; doi:

data_4030267
_publ_section_title
;
 Synthesis and structure of new
 n5-pentamethylcyclopentadienyldimethylplatinum (IV) complexes
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              599
_journal_page_last               615
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'C12 H21 Cl Pt'
_chemical_formula_weight         395.85
_space_group_IT_number           11
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.21(4)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.922(2)
_cell_length_b                   11.286(3)
_cell_length_c                   8.713(2)
_cell_volume                     673.7(3)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_crystal_density_diffrn    1.95
_refine_ls_number_reflns         1226
_refine_ls_R_factor_gt           0.041
_refine_ls_wR_factor_gt          0.050
_cod_data_source_file            EJSSIC-1990-27-599-615.cif
_cod_data_source_block           C12H21ClPt
_cod_original_sg_symbol_H-M      'P 21/m'
_cod_database_code               4030267
New quaternary lanthanoid transition metal arsenides with Ho5Ni19P12-type derivative structure
Pivan, J. Y.; Guerin, R.; Pena, O.; Padiou, J.; El Ghadraoui, E. H.; Rafiq, M.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 617–631; doi:

data_4030268
_publ_section_title
;
 New quaternary lanthanoid transition metal arsenides with Ho5Ni19P12-type
 derivative structure
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              617
_journal_page_last               631
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'As12 Ce5 Ni15 Zr3'
_chemical_formula_weight         2753.97
_space_group_IT_number           189
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      189
_symmetry_space_group_name_Hall  'P -6 -2'
_symmetry_space_group_name_H-M   'P -6 2 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   12.740(5)
_cell_length_b                   12.740(5)
_cell_length_c                   3.932(1)
_cell_volume                     552.7(3)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    42.64
_exptl_crystal_density_diffrn    8.28
_refine_ls_number_parameters     46
_refine_ls_number_reflns         526
_refine_ls_R_factor_gt           0.042
_refine_ls_wR_factor_gt          0.044
_cod_data_source_file            EJSSIC-1990-27-617-631-1.cif
_cod_data_source_block           Ce5Zr3Ni15As12
_cod_original_cell_volume        552.7(5)
_cod_database_code               4030268
New quaternary lanthanoid transition metal arsenides with Ho5Ni19P12-type derivative structure
Pivan, J. Y.; Guerin, R.; Pena, O.; Padiou, J.; El Ghadraoui, E. H.; Rafiq, M.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 617–631; doi:

data_4030269
_publ_section_title
;
 New quaternary lanthanoid transition metal arsenides with Ho5Ni19P12-type
 derivative structure
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              617
_journal_page_last               631
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'As12 Er5 Ni16 Zr3'
_chemical_formula_weight         2948.04
_space_group_IT_number           189
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      189
_symmetry_space_group_name_Hall  'P -6 -2'
_symmetry_space_group_name_H-M   'P -6 2 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   12.651(1)
_cell_length_b                   12.651(1)
_cell_length_c                   3.820(1)
_cell_volume                     529.47(15)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    53.387
_exptl_crystal_density_diffrn    9.246
_exptl_crystal_F_000             1304
_refine_ls_number_parameters     23
_refine_ls_number_reflns         464
_refine_ls_R_factor_gt           0.049
_refine_ls_wR_factor_gt          0.057
_cod_data_source_file            EJSSIC-1990-27-617-631-2.cif
_cod_data_source_block           Er5Zr3Ni16As12
_cod_original_cell_volume        529.47(19)
_cod_database_code               4030269
Crystal structure of Na2BaFe4F12 : a new ordered perovskite-like fluoride
Darriet, J.; Mayorga, S. G.; Tressaud, A.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 783–790; doi:

data_4030270
_publ_section_title
;
 Crystal structure of Na2BaFe4F12 : a new ordered perovskite-like fluoride
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              783
_journal_page_last               790
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'Ba F12 Fe4 Na2'
_chemical_formula_weight         634.66
_space_group_IT_number           204
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      204
_symmetry_space_group_name_Hall  '-I 2 2 3'
_symmetry_space_group_name_H-M   'I m -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.075(2)
_cell_length_b                   8.075(2)
_cell_length_c                   8.075(2)
_cell_volume                     526.5(2)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    9.291
_exptl_crystal_density_diffrn    4.003
_exptl_crystal_F_000             580
_refine_ls_number_parameters     14
_refine_ls_number_reflns         152
_refine_ls_R_factor_gt           0.0257
_refine_ls_wR_factor_gt          0.0250
_cod_data_source_file            EJSSIC-1990-27-783-790.cif
_cod_data_source_block           Na2BaFe4F12
_cod_original_cell_volume        526.5(4)
_cod_database_code               4030270
Crystal structure of Cu(1+3x)Bi(5-x)X8 (X = S, Se) alloys
Liautard, B; Garcia, J. C.; Brun, G.; Tedenac, J. C.; Maurin, M.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 818–830; doi:

data_4030271
_publ_section_title
;
 Crystal structure of Cu(1+3x)Bi(5-x)X8 (X = S, Se) alloys
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              818
_journal_page_last               830
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'Bi4.8 Cu1.6 S8'
_chemical_formula_weight         1361.3
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                85.08(3)
_cell_angle_beta                 81.99(3)
_cell_angle_gamma                73.05(3)
_cell_formula_units_Z            1
_cell_length_a                   4.029(1)
_cell_length_b                   6.906(3)
_cell_length_c                   12.902(5)
_cell_volume                     339.7(2)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    13.60
_exptl_crystal_density_diffrn    6.67
_refine_ls_number_reflns         977
_refine_ls_R_factor_gt           0.053
_refine_ls_wR_factor_gt          0.078
_cod_data_source_file            EJSSIC-1990-27-819-830-1.cif
_cod_data_source_block           Cu-Bi-Se
_cod_database_code               4030271
Crystal structure of Cu(1+3x)Bi(5-x)X8 (X = S, Se) alloys
Liautard, B; Garcia, J. C.; Brun, G.; Tedenac, J. C.; Maurin, M.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 818–830; doi:

data_4030272
_publ_section_title
;
 Crystal structure of Cu(1+3x)Bi(5-x)X8 (X = S, Se) alloys
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              818
_journal_page_last               830
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'Bi4.8 Cu1.6 Se8'
_chemical_formula_weight         1736.46
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                85.45(2)
_cell_angle_beta                 81.25(2)
_cell_angle_gamma                73.26(2)
_cell_formula_units_Z            1
_cell_length_a                   4.148(1)
_cell_length_b                   7.182(2)
_cell_length_c                   13.388(4)
_cell_volume                     377.23(18)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    25.06
_exptl_crystal_density_diffrn    7.61
_refine_ls_number_reflns         975
_refine_ls_R_factor_gt           0.053
_refine_ls_wR_factor_gt          0.076
_cod_data_source_file            EJSSIC-1990-27-819-830-2.cif
_cod_data_source_block           Cu-Bi-Se
_cod_database_code               4030272
Harbrecht, B.; Kushauer, J.; Weber, H.-J.; European Journal of Solid State and Inorganic Chemistry 27 (1990) 831–843; doi:

data_4030273
_publ_section_title
;
 
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              831
_journal_page_last               843
_journal_volume                  27
_journal_year                    1990
_chemical_formula_sum            'Ge8 K2 O17'
_chemical_formula_weight         931.08
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      62
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.371(2)
_cell_length_b                   8.800(1)
_cell_length_c                   13.372(3)
_cell_volume                     1573.4(5)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           AgK\a
_diffrn_radiation_wavelength     0.56
_exptl_absorpt_coefficient_mu    8.22
_exptl_crystal_density_diffrn    3.931
_exptl_crystal_F_000             1720
_refine_ls_number_parameters     134
_refine_ls_number_reflns         2408
_refine_ls_R_factor_gt           0.031
_refine_ls_wR_factor_gt          0.038
_cod_data_source_file            EJSSIC-1990-27-831-843.cif
_cod_data_source_block           K2Ge8O17
_cod_database_code               4030273
Synthesis, characterization and crystal structure of the new clathrasil phase octadecasil
Caullet, P.; Guth, J. L.; Hazm, J.; Lamblin, J. M.; Gies, H.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 345–361; doi:

data_4030274
_publ_section_title
;
 Synthesis, characterization and crystal structure of the new clathrasil
 phase octadecasil
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              345
_journal_page_last               361
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'C14 H24 F2 N2 O40 Si20'
_chemical_formula_weight         1460.04
_space_group_IT_number           87
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      87
_symmetry_space_group_name_Hall  '-I 4'
_symmetry_space_group_name_H-M   'I 4/m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   9.194(2)
_cell_length_b                   9.194(2)
_cell_length_c                   13.396(4)
_cell_volume                     1132.4(5)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_exptl_absorpt_coefficient_mu    0.612
_exptl_crystal_density_diffrn    1.873
_refine_ls_number_reflns         585
_refine_ls_R_factor_gt           0.0613
_refine_ls_wR_factor_gt          0.0394
_cod_data_source_file            EJSSIC-1991-28-345-361.cif
_cod_data_source_block           octadecasil
_cod_original_cell_volume        1132.4(6)
_cod_database_code               4030274
Synthesis and ionic conductivity of Rb(MoSb)O6
Garcia-Martin, S.; Veiga, M. L.; Jerez, A.; Pico, C.; Santamaria, J.; Gonzalez-Diaz, G.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 363–371; doi:

data_4030275
_publ_section_title
;
 Synthesis and ionic conductivity of Rb(MoSb)O6
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              363
_journal_page_last               371
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'Mo O6 Rb Sb'
_chemical_formula_weight         399.16
_space_group_IT_number           227
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.2556(1)
_cell_length_b                   10.2556(1)
_cell_length_c                   10.2556(1)
_cell_volume                     1078.657(18)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.542
_exptl_absorpt_coefficient_mu    68.511
_exptl_crystal_density_diffrn    4.916
_exptl_crystal_density_meas      4.91
_refine_ls_R_I_factor            0.029
_cod_data_source_file            EJSSIC-1991-28-363-371.cif
_cod_data_source_block           Rb(MoSb)O6
_cod_original_cell_volume        1078.66(3)
_cod_original_sg_symbol_H-M      'F d -3 m'
_cod_database_code               4030275
A combined X-ray and neutron powder diffraction study of K(Ti0.5Sn0.5)OPO4
Crennell, S. J.; Owen, J. J.; Cheetham, A. K.; Kaduk, J. A.; Jarman, R. H.; European Journal of Solid State and Inorganic Chemistry 28 (1991) 397–407; doi:

data_4030276
_publ_section_title
;
 A combined X-ray and neutron powder diffraction study of
 K(Ti0.5Sn0.5)OPO4
;
_journal_name_full
'European Journal of Solid State and Inorganic Chemistry'
_journal_page_first              397
_journal_page_last               407
_journal_volume                  28
_journal_year                    1991
_chemical_formula_sum            'K O5 P Sn0.5 Ti0.5'
_chemical_formula_weight         233.36
_space_group_IT_number           33
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      33
_symmetry_space_group_name_Hall  'P 2c -2n'
_symmetry_space_group_name_H-M   'P n a 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.9764(3)
_cell_length_b                   10.6461(2)
_cell_length_c                   6.4669(1)
_cell_volume                     893.39(3)
_diffrn_ambient_temperature      293
_diffrn_radiation_probe          neutron
_diffrn_radiation_type           white
_exptl_crystal_density_diffrn    3.474
_refine_ls_goodness_of_fit_all   2.089
_refine_ls_number_parameters     92
_cod_data_source_file            EJSSIC-1991-28-397-407.cif
_cod_data_source_block           K(Ti0.5Sn0.5)OPO4
_cod_original_cell_volume        893.38(2)
_cod_database_code               4030276